General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.85 g/cm³ Show Material materials with Density of 7.85 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa | |

20.0 °C | 212 GPa Show Material materials with Elastic modulus of 212 GPa | ||

100.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa | ||

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | ||

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | ||

400.0 °C | 184 GPa Show Material materials with Elastic modulus of 184 GPa | ||

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | ||

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | ||

Elongation | 20.0 °C | 25 % Show Material materials with Elongation of 25 % | |

Elongation, transverse | 20.0 °C | 23 % Show Material materials with Elongation, transverse of 23 % | |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

Shear modulus | 23.0 °C | 82 GPa Show Material materials with Shear modulus of 82 GPa | Typical for Low Carbon Steel |

Tensile strength | 20.0 °C | 340 - 460 MPa Show Material materials with Tensile strength of 340 - 460 MPa | |

Tensile strength, transverse | 20.0 °C | 340 - 460 MPa Show Material materials with Tensile strength, transverse of 340 - 460 MPa | |

Yield strength | 20.0 °C | 225 MPa Show Material materials with Yield strength of 225 MPa | |

Yield strength, transverse | 20.0 °C | 225 MPa Show Material materials with Yield strength, transverse of 225 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | |

20.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | ||

100.0 °C | 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.25E-5 1/K | ||

200.0 °C | 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.3E-5 1/K | ||

300.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | ||

400.0 °C | 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.41E-5 1/K | ||

500.0 °C | 1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 1/K | ||

600.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | ||

Unlock all property charts | |||

Max service temperature | 500 °C Show Material materials with Max service temperature of 500 °C | Typical for Carbon Steel | |

Melting point | 1480 - 1526 °C Show Material materials with Melting point of 1480 - 1526 °C | Typical for Low Carbon Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | ||

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | ||

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | ||

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | ||

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | ||

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | ||

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 56.9 W/(m·K) Show Material materials with Thermal conductivity of 56.9 W/(m·K) | |

100.0 °C | 56.4 W/(m·K) Show Material materials with Thermal conductivity of 56.4 W/(m·K) | ||

200.0 °C | 53.5 W/(m·K) Show Material materials with Thermal conductivity of 53.5 W/(m·K) | ||

300.0 °C | 49.4 W/(m·K) Show Material materials with Thermal conductivity of 49.4 W/(m·K) | ||

400.0 °C | 45.2 W/(m·K) Show Material materials with Thermal conductivity of 45.2 W/(m·K) | ||

500.0 °C | 41.3 W/(m·K) Show Material materials with Thermal conductivity of 41.3 W/(m·K) | ||

600.0 °C | 37.6 W/(m·K) Show Material materials with Thermal conductivity of 37.6 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 15.7 mm²/s Show Material materials with Thermal diffusivity of 15.7 mm²/s | |

100.0 °C | 14.5 mm²/s Show Material materials with Thermal diffusivity of 14.5 mm²/s | ||

200.0 °C | 12.9 mm²/s Show Material materials with Thermal diffusivity of 12.9 mm²/s | ||

300.0 °C | 11.2 mm²/s Show Material materials with Thermal diffusivity of 11.2 mm²/s | ||

400.0 °C | 9.6 mm²/s Show Material materials with Thermal diffusivity of 9.6 mm²/s | ||

500.0 °C | 7.9 mm²/s Show Material materials with Thermal diffusivity of 7.9 mm²/s | ||

600.0 °C | 6.3 mm²/s Show Material materials with Thermal diffusivity of 6.3 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.83E-7 Ω·m Show Material materials with Electrical resistivity of 1.83E-7 Ω·m |

100.0 °C | 2.27E-7 Ω·m Show Material materials with Electrical resistivity of 2.27E-7 Ω·m | |

200.0 °C | 2.95E-7 Ω·m Show Material materials with Electrical resistivity of 2.95E-7 Ω·m | |

300.0 °C | 3.8E-7 Ω·m Show Material materials with Electrical resistivity of 3.8E-7 Ω·m | |

400.0 °C | 4.81E-7 Ω·m Show Material materials with Electrical resistivity of 4.81E-7 Ω·m | |

500.0 °C | 5.99E-7 Ω·m Show Material materials with Electrical resistivity of 5.99E-7 Ω·m | |

600.0 °C | 7.38E-7 Ω·m Show Material materials with Electrical resistivity of 7.38E-7 Ω·m | |

Unlock all property charts |

Magnetic

Property | Value | Comment |
---|---|---|

Curie temperature | 770 °C Show Material materials with Curie temperature of 770 °C | Typical for Low Carbon Steel |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.02 % Show Material materials with Aluminium of 0.02 % |

Carbon | 0.17 % Show Material materials with Carbon of 0.17 % |

Manganese | 0.4 % Show Material materials with Manganese of 0.4 % |

Phosphorus | 0.03 % Show Material materials with Phosphorus of 0.03 % |

Silicon | 0.35 % Show Material materials with Silicon of 0.35 % |

Sulfur | 0.025 % Show Material materials with Sulfur of 0.025 % |